Materials Science and Metallurgy Engineering, 2017, Vol. 4, No. 1, 1-15 Available online at http://pubs.sciepub.com/msme/4/1/1
©Science and Education Publishing DOI:10.12691/msme-4-1-1
Behind the Development of Advanced High Strength
Steel (AHSS) Including Stainless Steel for Automotive
and Structural Applications - An Overview
Department of Metallurgical and Materials Engineering, Indian Institute of Technology Roorkee *Corresponding author: firstname.lastname@example.org, email@example.com
AbstractSafety is paramount importance along with enhancing fuel efficiency of the transport car over the last three decades. Advanced high strength steels play a pivotal role towards achieving the desired structural characteristics of the motor vehicles. Many structural components have been replaced by advanced high strength steels like IF steel, Bake hardening steel, HSLA steel, Micro alloyed steel, Dual Phase steel, Ferrite Bainite steel, Martensitic steel, Hot formed steel, TRIP steel, TWIP steel etc. along with austenitic and ferrite grade stainless steels due to its superior strength and ductility. In the current context it has been attempted to see the causes behind the development of those mentioned steels from conventional to third generation as well the strengthening mechanisms employed towards the development of advanced high strength structural steels. It has been observed from literature study that substantial development have been progressed from metallurgical point of view in this matter over the last decade.
Keywords: advanced high strength steel, automotive, strengthening mechanism, stainless steels
Cite This Article:Debasish Chatterjee, “Behind the Development of Advanced High Strength Steel (AHSS)
Including Stainless Steel for Automotive and Structural Applications - An Overview.” Materials Science and
Metallurgy Engineering, vol. 4, no. 1 (2017): 1-15. doi: 10.12691/msme-4-1-1.
1. Background towards Development of
Advanced High Strength Steel (AHSS)
Including Stainless Steel
Modern Automotive market demand improvement of fuel efficiency and simultaneously reduction of green house gas emission by lowering the vehicle weight due to the stringent requirement of reducing green house gas
emission throughout the world . In recent years the
function require in automobile industry is diverse. In addition to comfort, high fuel efficiency, emission control and safety are also important part to make a vehicle. These goals are possible to achieve by lowering the vehicle kerb weight and simultaneously improving the crash worthiness behavior of body parts of the automobile . As a result development of more reliable advanced high strength steels are required to manufacture for body parts of vehicle. Over the last three decades aluminum and magnesium grade steels and conventional high strength steel use for passenger safety in the vehicle. Reliability of automotive parts can be enhanced by using advanced high strength steel (AHSS). Characteristics of this steel are good formability and toughness. Broadly dual phase steel, transformation induced plasticity steel, complex phase steel and martensitic steel are under AHSS. The advanced high strength steel generally have yield strength greater than 300 MPa and ultimate tensile strength will be greater
than 600 MPa . By applying AHSS merely 203 kg, 25
percent weight of the vehicle can be reduced by using thinner high tensile and formable steel as reported in
ULSAB study . The terms “High-Strength” and
“Advanced High-Strength” steels are differ in the sense that AHSS steel is more superior in terms of mechanical characteristics than HSS (Interstitial free steel, Bake hardened steel, high strength low alloy steel). When tensile strength exceeds 780 MPa called “Ultra High Strength Steel” .
Over the last four decades metallurgists are trying to develop advanced high strength and ductility steels for transport and structural purposes. Some parts of the sports cars are frequently made by aluminum and magnesium like low density materials. Normal stainless steel exhibit tensile properties approximately 327 MPa yield strength, high strength steel like S420MC grade shows 440 MPa 0.2% offset yield strength, TRIP700 steel yield strength is 495 MPa and advanced high strength steel like DP1000 (Dual Phase steel) have 922 MPa, MS1200 (martensitic steel) have 1238 MPa yield strength properties
respectively . More advanced high strength contain
steels are desperately use in many automotive parts to
further reduce the weight of the vehicle . TWIP
ductility third generation steel which will be less costly than second generation high strength steel like TWIP .
Quench and partitioning thermomechanical treatments are recent techniques to develop third generation advanced high strength steel by grain refinement with precipitation
hardening [11,12,13]. Ultra grain refinement exhibit
advanced high strength steel structure properties like
superior strength , good low temperature toughness
 and high stretch formability . These
nano-crystalline structures produce grains lower than 100 nm
. It is targeted by the researchers to develop more ultra fine grains structure by thermomechanical treatments to get superior strength properties in the future advanced structural grade steels. In the strategic research agenda of European Steel Technology Platform (ESTEP) it was stated that advanced high strength steel with moderate ductility have to be developed within the year 2030 including austenitic stainless steel for future generation light weight and safe vehicle by thermomechanical treatments instead of incorporating costly alloying elements . Gradually global demand CO2 emission
reduction more high strength and ductile chassis and body in white (BIW) structure is required for automotive purpose which has developed a big market for austenitic grade steel to manufacture transport vehicle along with
many structural components of automotive body .
Recent market is moving towards sustainability and reduction of green house gases and less emission of other noxious gases by using stainless steel made public transport like rail or metro rail rather than extensive use of automotive vehicles due to its safety, less maintenance and consistently generating a green pollution free environment in the nature . Along with good corrosion resistance of stainless steels (Austenitic and duplex stainless steel), it shows excellent toughness (25.9 – 38.0 J/g) as compared to other high strength steel like HSLA steel (12.5 J/g) and simultaneously produce good formability and fatigue properties which are essential for crashworthiness purposes for car safety applications . So recent trend is to develop advanced high strength future generation structural stainless steel along with other grades of steels by decreasing alloying element by purposefully incorporating nitrogen content in the austenitic grade steel as well changing the microstructure by applying advanced thermomechanical treatments.
2. Role of Various Strengthening
Mechanisms towards Development of
Advanced High Strength Structural
European commission of steel platform has set target to develop high strength with moderate ductility steel within the year 2030. According to commission high strength and moderate ductile steel have to be developed for automobile industry. Not only that high strength austenitic stainless have to be developed for structural and rail coach manufacturing purpose for better safe life of human being. In this regard it is essential to know various strengthening
mechanisms to better understand the physics behind development of superior strength and elongation advanced high strength steel (AHSS).
Grain Boundary Strengthening by Generation of Ultra Fine Grains Structure: - Generation of ultra fine grain is a popular method to develop high strength steel. Not only grain refinement the increasing misorientation angle across grain boundaries increases the yield strength of the material . A normal relation between grain size and yield strength proposed by Hall-Petch is as follows:-
0 i k d( )
σ =σ + − σ0 – Yield Strength of Fine grain Material
σi – Friction Stress of the material or Initial yield Strength
k – Locking parameter due to hardening from grain boundary
d – Grain diameter (mm).
Hall Petch behavior has been explained by various models like pile up model, dislocation density model and
composite model . The basic thinking of pile up
model is to consider the concentration of huge number dislocations along the grain boundaries causing retardation of dislocation movement and enhancement of yield strength property of the steel.
Dislocation Strengthening by Severe Plastic Deformation Particularly for Austenitic Grade Stainless Steels: - The yield strength of austenitic stainless steel can be drastically improved by generation of plasticity and metastable phase transformation introducing severe plastic deformation . Austenitic steel generally posses’ high ductility with low yield strength and has very good strain hardening property due to its low stacking fault energy. Due to low stacking fault energy the dislocation dissociated to two Shockley partial dislocations which require stress to collide those partial dislocations before movement of united perfect dislocation through slip plane which causes high strain hardening rate of this type of steel. Strain induced hardening is achieved due to obstacles of movement to large number of dislocations and interaction of dislocations with martensite phase which generate during severe plastic deformation. Stacking fault energy (SFE) dictate formation of shear bands which ultimately act as a nucleation site for formation of α' martensite. Plastic deformation not only develop high hard martensitic phase but simultaneously improve the yield strength due to formation of twins, shear bands, dislocations and Suzuki locking. The cold work metal contain more dislocations (approximately 1010 mm2) as compare to annealed steel (contain in the range of 104 to 106 per mm2) .
Materials Science and Metallurgy Engineering 3
Figure 1. (a) Changes of Tensile Strength with increasing Ni content in the Copper- Nickel Alloy (b) Schematic diagram of generation of Lattice strain with incorporation of small substitutional element within the metal (Reprinted from )
Figure 2. Orowan mechanism of strengthening the metal matrix from precipitates (Reprinted from ) Strengthening the Metal by Strain Ageing
Treatments:- Bake hardening is a typical static strain ageing treatment which is generally applied to improve the tensile properties of all types of steels. Typically below 2000C temperature with sufficient time heating are applied to cold work stainless, dual phase, transformation induced plasticity steel to improve the yield strength as high as
maximum 200 MPa . Strain aging increase the yield
strength and simultaneously decrease the ductility also and nitrogen plays a pivotal role in static strain aging due to its higher solubility and diffusion coefficient as mentioned in the literature . Yield point phenomena observed for static strain ageing and dynamic strain ageing produce serrated stress strain curve and sometimes generation of twins and stress assisted martensite also produced that behavior of mechanical properties of steel.
Precipitation hardening of Steel: - Very fine second phase particles precipitation on the base metal matrix improve the mechanical properties of steel. Precipitation of cementite particles from ferrite occurs during ageing
treatments by nucleation and growth process .
Precipitation and dispersion strengthening mechanism has
been studied by researchers and it is observed that Orowan
dislocation bypassing mechanism (shown in Figure 2)
play a pivotal role in this regard .
Recovery, Recrystalization, Grain Growth and Annealing mostly apply to strengthen austenitic grade stainless steels:- After cold working of austenitic grade stainless steel when subjected to annealed elevated temperature (above 0.5Tm) is undergone recovery (relieve of internal stress without application of any external pressure due to dislocation motion) for short time annealing, followed by recrystalization (generation of new equal size strain free grains) for certain period of annealing treatments and finally grain growth (formation of large size grains from new strain free grains) for long period of annealing at elevated temperatures [25,28,29,30].
3. Development of Conventional High
improving the rigidity of the vehicle several high strength steels have been used throughout the last two decades. Generally conventional steel used for structural application are mild steel, IF (interstitial free) steel, BH (bake hardened) steel and micro alloyed or HSLA (high strength low alloy) steel. But conventional steels have major disadvantages is its heavy weight which is the barrier for reduce fuel consumption .
IF (Interstitial Free) Steel: - This steel was first invented in Japan at the end of the year 1960 . The Interstitial Free steel generally used for making rear floor pan, spare wheel well and front-rear door inners which is shown in Figure 3 . But the biggest disadvantage of this steel is its low tensile strength less than 360 MPa . Upto 450 MPa tensile strength improvement has been achieved for this steel by solid solution strengthening . By addition of 1.2% Cu the yield strength and tensile strength value around 460 MPa and 575 MPa respectively achieved by precipitation hardening . Ultra fine grain structure using equal-channel angular extrusion/pressing (ECAE/P) method and annealing were applied for this
steel recently [37,38]. 708-900 MPa tensile properties
with nearly 15%-10% ductility observed for this steel by
this thermomechanical method [39,40]. Ultrafine grain
structure by cold rolling and annealing with bake hardening together improves toughness and elongation of this steel [41,42,43].
Bake hardening Steel: - This steel mostly has ferrite microstructure. Denting problems in automotive outer body panels can be avoided by uses of Bake harden (BH) Steel. Due to lack of movement of dislocations by interstitial atoms bake harden steels after painting or static strain aging posse’s very high strength with superior ductility and after bake hardening of a pre-strain cold rolled continuous annealed steel it is possible to improve the yield strength 10 – 54 MPa and work harden ability
around 17-82 MPa depending on the panel location .
Normally bake hardening treatment is given to low carbon steel and IF steel. But now a days due to great formability of IF steel most panel is made by IF-BH steel.
High Strength Low Alloy Steel (HSLA):- This category of steel extensively used for making body parts, wheels, and ancillary parts, suspension and chassis components in vehicle application due to its yield strength
greater than 275 MPa . The HSLA steel first
developed in the year 1960 . Different types of HSLA steels are available in market like weathering steel, micro alloyed steel, as-rolled pearlitic steel, low carbon bainite steel, dual phase steel and inclusion shape controlled steel. Minimum yield strength approximately 550 MPa was achieved by precipitation hardening and ferrite grain
refinement (less than 3 µm) [46,47]. To improve the
properties of HSLA steel various alloying elements has been added like Nb, Ti, V and boron. 550 MPa yield strength and 20% elongation at room temperature was possible to get by TiN precipitates and increase percentage of fine bainite and generation of uniformly distribute metal carbides in the matrix [48,49].
Micro-alloyed Steels: - It is basically containing niobium, vanadium, titanium, zirconium and boron is used for discrete automotive parts like power train, suspension component systems due to its excellent strength and toughness by formation of fine grain size with
carbo-nitrides precipitate in the ferrite matrix by thermomechanical treatements along with accelerated cooling process shows around 400-800 MPa yield strength and 500-1000 MPa ultimate tensile strength steel along
with 23-26% elongation [50,51,52]. High strength
microalloyed steels are extensively (around 60%) used to
manufacture auto body . In heavy duty truck wheel
disc and wheel rims instead of conventional mild steel hot rolled microalloyed steel is extensively using to take the high compressive strength with safety as 90% 5µm polygonal ferrite and 10% pearlite formed with 570 MPa yield strength, 610 MPa tensile strength and 26%
elongation . Due to pinning effect Nb improves the
tensile strength of this steel from 970 MPa to 1200 MPa
but simultaneously lower the ductility nearly 4% .
Thermomechanical treatments with 1%-2% Cu addition enhance the tensile properties to 1364-1403 MPa with 11%-14% ductility [56,57].
Generation Advanced High Strength
Steels for Vehicle Components
In recent decade metallurgists are trying to develop more high strength with superior ductility steel than the conventional high strength steel known as advanced high strength steel (AHSS). The microstructure of this type of steel is multi phase and complex in nature. The percentage use of conventional high strength steel (HSS) and advanced high strength steel (AHSS) for the year 2007 and 2015 is shown in Figure 4 (a) as well as it is observed that the use of AHSS will increase for future steel vehicle
depicted in Figure 4 (b). Generally all types of AHSS
produce by changing the chemical composition of steel and advanced cooling treatment from austenite phase or austenite + ferrite phase.
Dual Phase Steel: - Dual phase steel consists of ferrite and martensite microstructure. This steel is extensively used to manufacture crumple zone to body structure of a vehicle, closures, hood, doors, front and rear rails, beams and cross members, rocker, sill, cowl inner and outer, crush cans, shock towers, fasteners and wheel also as the yield strength and ductility of this steel can be controlled in a broad range by controlling hot coiling and bake
hardening temperature . In recent years most of the
automotive parts are replaced by dual phase steel rather than use of conventional HSLA steel. Dual phase steels have typical yield strength and tensile strength value ranging from 210 MPa-1150 MPa and 440-1270 MPa with elongation nearly 35% -10% for DP 210/440 grade to
DP 1150/1270 grade respectively [58,59]. Ultra high
Materials Science and Metallurgy Engineering 5
Figure 3. Inner door body panel for automobile from IF steel (Reprinted from )
Figure 4. (a) Comparison of HSS and AHSS from past and present (b) Future Steel vehicle (FSV) & Battery Electric Vehicle (BEV) (Reprinted from
TRIP (Transformation Induced Plasticity) Steel: -Development of advanced high strength steel is a challenge for automotive industry for making fuel efficient, less emission and safe vehicle for passengers over the past decade or so. It has been targeted by metallurgical researchers to develop more complex microstructure steel with superior performance in terms of strength and ductility. The commercially developed dual phase steel usually consists of ferrite and martensite microstructure which has been discussed earlier and on the other hand TRIP steel shows a ferrite-bainite-retained austenite and martensite microstructure. Due to presence of high amount C and Si, 70% polygonal ferrite with grain size in the range of 1.5-4 µm and nearly 20% retained austenite along with remaining bainite plus martensite mixture observed for this steel . TRIP steel used for making frame rails, rail reinforcement, side rail, crash box, dash panel, roof rails, B-pillar upper, engine cradle, front and rear rails, seat frame, bumper cross member etc as
depicted in the Figure 5 . Lamellar austenite with
bainitic ferrite structure improves the mechanical properties to UTS level 682 MPa and elongation 70% . Intercritically treated at 630°C of this steel possess 800
MPa strength and 29% ductility . TRIP steel was
intercritically annealed at 600°C and 650°C which shows nearly 1200 MPa and 1400 MPa true stress with 0.3 and 0.1 true strains respectively . High stretch-flangeability (UTS 980-1470 MPa and elongation 25-10%) automotive components like reinforcement, sheet frame were developed by NbC precipitation with TRIP effect . A New TBF steel (TRIP steel with bainitic-ferritic matrix)
shows high toughness value (100-120 J/cm2) as well as
low ductile-brittle transition temperature (range of -130°C to -150°C) and ultimate tensile strength of 1527 MPa, ductility 13.4% . High strength (approximately 1000 MPa) with high elongation (nearly 40%) steel was produced by 36% cold rolled and intercritically annealed
at 640°C for 1 hour . By alloying Mo, Nb and Mn it
has been possible to produce ultra high strength (1000 MPa-1400 MPa) and high ductility (35%-13%) of these
steels [83,84]. Tramp elements improve ductility and
simultaneously hydrogen absorption during white painting is a critical problem to crack initiation of this advanced high strength steel [85,86].
Complex Phase (CP) Steel: -The complex phase steel
is a fine grain structure with mixture of martensite, retained austenite and pearlite within the ferrite-bainite matrix and applicable for manufacture of different automotive components like frame rails, chassis components, transverse beams, B-pillar, tunnel stiffener, rear suspension brackets, fender beam, rear frame rail reinforcements, rocker outer, rocker panels, bumper beams etc as its tensile strength within the range of 800-1470 MPa and elongation 15-5% which is higher than DP steel as embodied in Figure 6[58,87].
Martensitic Steel (MS):- Martensitic steel is a great innovation of metallurgist which consists of small amount of ferrite-bainite mixture in fully martensitic matrix due to high cooling rate from quenching and posses extremely high strength in the range of 1200 MPa to 1500 MPa with elongation approximately 8%-5% which is mainly used for many automotive parts like cross-members, side intrusion beams, bumpers beams, bumpers reinforcements,
rocker outer, side intrusion beams etc [58,88]. Auto
tempering of the lath martensite is the cause of high strength of this steel [89,90].
Ferritic-Bainitic Steel: - Ferritic-Bainitic steel is a special case of application particularly for rim; brake pedal arm, seat cross member, suspension arm, lower control arm, bumper beam, chassis parts and rear twist beam etc as depicted in the Figure 7[91,92]. Mo addition improves mechanical properties of this steel as it promotes more bainite formation which in the range of 1100 MPa-1200 MPa and 18-22% respectively whereas the base steel shows tensile strength in between 700-800 MPa and nearly 22% ductility . Banitic hardening by nano scale (Nb,Ti)C precipitates produced by metallurgists for
automotive wheel application . Cold rolled and
continuous annealing carbide free ferritic banitic steel is a new type of steel which shows a greater formability than the martensitic steel or dual phase steel with same ultimate
tensile strength (in the range of 1200-1500 MPa) .
Cementite free optimum bainitic structure usually consist of upper bainitic-ferrite, carbon enriched retained austenite and some martensite with exceptionally high tensile strength (in the range of approximately 1600-1950 MPa) and total elongation over 10% obtained by FRT (finishing rolling temperature) at 9300C followed by FCT (finishing coiling temperature) in between 550°C-650°C
Materials Science and Metallurgy Engineering 7
Figure 6. (a) Seat Flange, (b) tunnel stiffener and (c) suspension arm made by CP 600,800 Steel (Reprinted from )
Figure 7. (a) FB 560 for suspension arm (b) FB 590 for wheel application (c) Front and rear under seat cross member made by FB 560 (d) FB 540 for uncoated suspension arm (Reprinted from )
Hot formed (HF) Steel: - This steel generally use for manufacturing automobiles structural and safety components due to its high tensile strength (approximately 1500 MPa) and ductility nearly 6% act as a high weight saving (30-50%) rather than use of conventional cold
rolled grade . Recently metallurgist are trying to
1623 MPa with ductility around 13.7% and impact energy nearly 60-70 J [98,99,100].
5. Birth of 2nd
Generation Advanced High
Strength Steel (AHSS)
TWIP (Twin Induced Plasticity Steel):- This steel contain deformation twins in austenite matrix with ultimate tensile strength (in the range of 900 MPa – 1200 MPa), elongation within 20% – 50% due to soft phase austenite with twin boundary act like grain boundary and typically applicable for manufacture of A-pillar, wheelhouse, front side member, lower control arm, front and rear bumper beams, B-pillar, wheel rim, floor cross
member, door impact beam etc of a vehicle . The
dislocations movements hinder from these deformed twins and low stacking fault this FCC alloy exhibit high tensile as well as ductile properties [101,102]. Nano grains TWIP steel shows approximately 1195-1330 MPa yield strength and formability in the range of 20.1-13.7% respectively
mainly used for anti-intrusion auto body parts .
Different percentage cold reduction with annealing produce fine grain (nearly 8 µm – 10 µm grain size) TWIP steel exhibit tensile strength nearly 800 MPa and ductility
close to 60% [104,105]. An extra ordinary high tensile
strength (nearly 1702 MPa) with high ductility (approximately 24%) were observed for TWIP steel containing Ni and Cr with high Mn and Si (0.61C–
22.3Mn–0.19Si–0.14Ni–0.27Cr) after deform severe plastically by Equal Channel Angular Pressing (ECAP) method by two passes at 300°C as well as 400°C (as received material shows closely 1000 MPa tensile strength and ductility above 120%) due to generation of deformation microbands (distance between two parallel microband is ≈260±37nm) and nano twins within the primary twins or micro twins in the ultra fine grains (0.3-0.6 µm as compare to 34 ± 21 µm austenite grains for as received material) as well as the formation of stacking faults (around 50µm in size) within the subgrains as embodied in the Figures 8 (a), (b) and (c) . TWIP steel has enough ductility so it is extensively use for crash worthiness purpose for absorbing impact energy. The generation of twin is important with deformation temperatures. It was found that it produce maximum quantity of twin with deformation at room temperature rather than at high temperature (like 4000C) and very low temperature like -150°C or cryogenic temperature (-196°C) and crash resistance super ductility TWIP steel has high value of specific absorption energy (0.5 j/mm3) than the conventional deep drawing steel like IF steel, bake hardening steel, other thermomechanically treated steels due to formation of extensive twins at high strain rate
. Recently ferritic-austenitic duplex light weight steel exhibit high tensile strength (734 MPa) and high elongation around 77% for generation of deformation induced martensite and twins within austenite grains simultaneously .
Materials Science and Metallurgy Engineering 9
Figure 9. (a) The Red region of “Banana Curve” showing the strength and ductility required for Carbon Steel including stainless steel for future generation Automotive Purposes (Reprinted from  ) (b) New Market for Austenitic Stainless Steel for Making Automobile Structural Parts (Reprinted from )
6. Towards Development of Future or 3rd
Generation Advanced High Strength
Third generation AHSS concept came from the research
gap found to develop 1st generation AHSS and 2nd
generation AHSS. The third generation steel consists of a mixture of martensite and austenite as austenite plays an important role in work hardening. So austenite stability at room temperature is important by controlling thermomechanical treatments. In this point of view “Q & P” treatments has play an important role to develop future generation advanced high strength steel. Quench and partitioning process controlled formation of retained austenite interspersed with partitioned martensite . Third generation AHSS consists of fine grain ferrite, carbide free bainite, martensite and retained austenite.
High volume percentage stable retained austenite is required to develop high strength and ductile materials. Nb microalloyed 0.17% C, 3% Mn, 1.5% Al, 0.2% Si, 0.2% Mo steel were thermomechanically processed in the temperature range of 400°C-450°C on the basis of DCCT (Deformation continuous cooling transformation) diagram which exhibit very fine grain bainite microstructure with nearly 20% stable retained austenite . Approximately 1650 MPa tensile strength and total elongation 20% achieved when 0.3C-4.0Mn-2.1Si, 1.5 Al, and 0.5 Cr steel is subjected to dual stabilization heat treatment (DSHT) which is basically a five stage cooling schedule act as a paraequlibrium carbon partitioning (different from quench and partitioning treatment) due to formation of
approximately 30 vol% stable retained austenite .
strength by “Q & P” treatments at 270°C and 400°C respectively due to generation of high volume fraction carbon enriched retained austenite . In recent decade along with quench and partitioning treatments, tempering were also applied to boron alloyed directly hot rolled steel to enhance better formability with high strength (nearly 2000 MPa) which has been attributed due to formation of nano carbide with dislocation density anhilation during
tempering . Quench partition and tempering
treatment (“Q-P-T”) also applied to a steel of composition Fe-0.6C-1.5Mn-1.5Si-0.6Cr-0.05Nb hot-rolled high-carbon steel which exhibit high tensile strength (approximately 1950 MPa) and high formability (around 12.4%) due to formation of high percentage retained austenite which absorb dislocation intensity and provide TRIP effect during deformation . A multiphase steel contain microstructure mixture of bainite, martensite and improved retained austenite (13%) were achieved by “Q & P” treatments to a Co containing steel (composition 0.32 C, 1.78 Mn, 0.64 Si, 1.75 Al, and 1.20 Co all in wt%) which shows high tensile strength ≈1470 MPa and high
total elongation ≈ 13% . Instead of “Q & P”
treatment hot stamping with bake hardening (HS-BH) treatments were applied a steel composition like Fe-0.39C-1.56Si-1.54Mn-0.98Ni-1.01Cr-0.45Mo-1.40Cu-0.028Ti-0.0023B-0.025Al shows nearly 2000 MPa tensile strength and approximately 18% formability due to formation of film like and blocky retained austenite with tempered lath like martensite and spherical nano size (≈ 15nm) Cu rich precipitates .
7. Focus to Develop Advanced High
Strength Stainless Steel for Future
For the last three decades materials for the various parts of the vehicle have been developed in the narrow hyperbolic regions of the “Banana Curve” (bottom region of the curve) depicted in Figure 9 (a) . Globally decrease CO2 emission is required for automotive purpose
which has increased the demand of austenitic stainless steel grade in the world market which has been depicted in the Figure 9 (b) . So it is necessary to look behind the developed advanced high strength stainless steels mechanical properties for use of structural and automotive components.
Thermal fatigue and high temperature strength of ferritic stainless steels were improved by Nb incorporated laves phase precipitation in exhaust engine components
. As Ultra High Strength Stainless Steel is highly
desirable for automotive, aerospace, nuclear, gear and bearing industries so alloy design is important by nano-particles along with lath martensite is precipitation within
the matrix . 630 MPa yield strength and ductility
approximately 70% AISI 304 austenitic stainless steel was developed by gradient nanostructure and dense deformation twins’ boundaries formation for dislocation blocker by Ultrasonic Nano-Crystal Surface Modification
technique . 60% CR and annealed at 800°C for 10
sec of AISI 201 austenitic steel shows 450 MPa to 800 MPa Y.S. and 900 MPa to 1100 MPa U.T.S. due grain
fineness to 1.5 µm level as well as elongation found 50% for fine grain and 70% for as received coarse grain
structure . High nitrogen and enhanced Mo contain
super austenitic stainless steel is used to make high speed passenger craft as well as duplex stainless steel typically used for making maintenance free bridge column and repeated use of AISI 316L steel for medical purposes
. So mechanical property improvement of stainless
steels are target by many metallurgists. High pressure torsion (HPT) technique produces approximately 1800 MPa tensile and nearly 10% ductility property of austenitic grade steel . 90% Cryorolling was applied to Fe-25Cr-20Ni grade austenitic stainless which exhibit approximately 1500 MPa tensile strength and 6.4%
ductility . Nano-crystaline (grain size 65nm) with
tensile strength 1485 MPa and elongation 33% AISI 201L was formed after 95% cold rolling and annealing at 850°C for 30 seconds . It is observed by the researchers that fine grains austenitic stainless steels shows excellent strength and ductility due to deformation twins and on the other hand coarse grain structure shows low strength with high ductility from strain induced martensitic
transformation . Increased retained austenite
(approximately 70%) after cold rolling produce very high strength (nearly 2236 MPa with 12.3% elongation) austenitic grade high nitrogen Ni-free steel . Three stages cold rolling and annealing were applied to develop ultra high strength (yield strength-1120 MPa and tensile strength-1440 MPa) with formability nearly 12% AISI 304 stainless steel due to generation of ultra fine austenite
grains in the range of 80-150 nm . Ultra high
strength (yield strength-740 MPa to 1290 MPa and ultimate tensile properties-1003 MPa to 1415 MPa and ductility 45.9% to 8.2%) ferritic-austenitic stainless steel was developed by fine dislocation structure, grain refinement
and partial recrystalization . Thermomechanical
treatments of low density duplex steel exhibit a unique property of strength and ductility (tensile strength-925.9
MPa and elongation- 50.2%) . It was observed that
pre-cooling induce high strength (1240 MPa) and high formability (42%) of high manganese austenitic steel
. A new Ni-free austenitic stainless steel was
designed which posses’ extremely high strength (2400 MPa) and extraordinary ductility (40%) due to slow martensite transformation with mechanical twins by solid solution and dislocation strengthen from high Mn and
Nitrogen . Sometimes only cold deformation also
produce as high as 1257 MPa yield strength, 1444 MPa ultimate tensile strength and nearly 2% total elongation
. Large strain severe plastic deformation applied to S304H austenitic grade stainless steel which exhibit superior tensile properties (nearly 2050 MPa) and elongation 5%-7% as compared to 290 MPa tensile strength with approximately 60%-61% formability of the as received material due to generation of deformation twin and dislocation intensity . Continuous heating of the cold rolled austenitic stainless steel produce 810 MPa yield strength, 1163 MPa ultimate tensile strength and
nearly 26% elongation property . Nb alloyed
nano/ultrafine grain AISI201 type austenitic grade steel shows excellent tensile and ductility (~ 1200 MPa Y.S.
and 1500 MPa U.T.S. with elongation 35%) .
Materials Science and Metallurgy Engineering 11
(Y.S. - 790MPa, U.T.S. - 1300 MPa, ductility – 28%)
produced by cold rolling and annealing . Oxide
dispersed bimodal ultra fine grain distributed high strength (1200 MPa yield strength) and moderate ductility (less than 10%) developed by mechanical alloying and hot isostatic pressing (HIP) . Around 1700 MPa tensile strength with 5% - 10% elongation contain 19Cr duplex stainless steel formed by cold rolling due to generation of high dislocations pile up at twin grain boundaries . New ultra high strength maraging stainless steel shows 1649 MPa Y.S., 1928 MPa U.T.S. and 10% elongation, strengthen by Ni, Cr, Mo precipitates after ageing . Another super high strength newly developed light weight austenitic stainless steel shows 1800 MPa tensile strength with 50% elongation due to containing low density Al and generations of twins during transformation of FCC austenite to BCC martensite at the time of tensile testing
. Cryorolling followed by annealing of AISI304L
stainless steel austenitic grade exhibit 1295 MPa tensile strength and approximately 20% ductility form bimodal
grains and twining effect . The drawback of AISI
301 austenitic stainless steel towards use for structural purpose is its low yield strength (250 MPa – 350 MPa) which can be improved by grain refinement using repeated cold rolling and annealing thermomechanical treatments upto as high as 1970 MPa . Quenching and Partitioning (Q&P) is a relatively new technique applied to AISI 420 martensitic stainless steel grade which exhibit nearly 1570 MPa U.T.S. and 15.7% elongation due to formation of twined martensite in the matrix . Recently ultra fine grain (270 nm) AISI 304 steel shows 1890 MPa Y.S. and 2050 MPa U.T.S. with 6% ductility .
From the detailed literature study it is readily observed that there is a vast demand of high strength and moderate ductile advanced stainless steel for future transport as well structural body manufacturing purpose. last 3 decades significant contribution exerted for developing advanced high strength steel like 1st generation steels which exhibit best tensile properties in the range of 800-1000 MPa yield strength, 1200 – 1600 MPa ultimate tensile strength with
20%-13% ductility. 2nd generations TWIP steel has
900-1700 MPa ultimate tensile strength and approximately 20% ductility. 3rd generation steels produce mechanical properties like maximum 2000 MPa ultimate tensile strength and nearly 18% of formability by hot stamping and bake hardening treatments. These advanced developed steels are frequently used for making automobile parts, body sheets, panels, and crash worthiness and for making several accessories. In recent decade austenitic grades steels make attention to the steelmaker for capturing structural and automobile market due to its superior corrosion property and subsequently enhanced mechanical properties. Nano/ultra fine grains AISI 201 steel which produces as high as 1200 MPa Y.S., 1500 MPa U.T.S. and approximately 35% ductility as a future steel. Low density austenitic grade steel with superior strength and ductility (nearly 500 MPA Y.S., 1800 MPa U.T.S. and 50% elongation) developed by twin assisted martensitic
transformation. European commission has targeted to develop new generation advanced high strength steel by 2030 which have strength and ductility within the so called banana curve.
The author is gratefully acknowledging the Ministry of Human Resource Development (MHRD) for providing research fund from Grant No MHR-02-23-200-429.
 Yoshitaka Okitsu, Fabrication of ultrafine grained steels without severe plastic deformation and their application in automotive structures, Graduate School of Engineering, Phd Thesis, Osaka University, 5-12, (2012).
 Sekita Takashi, Kaneto Shuji, Hasuno Sadao, Sato Akio, Ogawa Takao, Ogura Kuniaki, Materials and Technologies for Automotive Use, JFE Technical Report, No. 2 , 1-18, (2004).  R. Kuziak, R. Kawalla, S. Waengler, Advanced high strength
steels for automotive industry, Archives of Civil and Mechanical Engineering, Vol. VIII, No. 2, 103-117, (2008).
 ULSAB program report, ULSAB Executive summary, Available at: http://www.worldautosteel.org, (2015), [Accessed October 2016].
 Carrie M. Tamarelli, AHSS 101: The Evolving Use of Advanced High-Strength Steels for Automotive Applications. Student’s intern report, summer, Materials Science and Engineering, University of Michigan, 1-45, Available at:
http://www.autosteel.org, (2011), [Accessed October 2016].  E. Silvestre n, J. Mendiguren, L. Galdos, E. Sáenz de Argandoña,
Comparison of the hardening behaviour of different steel families: From mild and stainless steel to advanced high strength steels, International Journal of Mechanical Sciences, 101-102, 10-20, (2015).
 H. Takechi, Transformation Hardening of Steel Sheet for Automotive Applications, The Journal of The Minerals, Metals & Materials Society, 60, No.12, 22-26, (2008).
 O. Grässel, L. Krüger, G. Frommeyer, L. W. Meyer, High strength Fe-Mn-(Al, Si) TRIP/TWIP steels development - properties – application, International Journal of Plasticity, 16, 1391-1409, (2000).
 David K. Matlock and John G. Speer, Third Generation of AHSS: Microstructure Design Concepts, Chapter 11: A. Haldar, S. Suwas, and D. Bhattacharjee (eds.), Microstructure and Texture in Steels, Springer, London, 185-205, (2009).
 F.G. Caballero, C. García-Mateo and J. Cornide, S. Allain, J. Puerta, M. Crouvizier, T. Mastrorillo, L. Jantzen, E. Vuorinen, L.E. Lindgren, K. Eriksson, G. Berglund, A. Hirvi, V. Lang, T.T. Nyo, P. Suikkanen, A.-J. Ristola, European Commissions Technical report (EUR 25977): New Advanced Ultra High Strength Bainitic Steels: Ductility and Formability (DUCTAFORM), 1-130, (2013).  J. G. Speer, D. V. Edmonds, F. C. Rizzo, D. K. Matlock,
Partitioning of carbon from supersaturated plates of ferrite, with application to steel processing and fundamentals of the bainite transformation, Current Opinion in Solid State and Materials Science, 8, 219-237, (2004).
 K. Sugimoto, M. Murata, S. M. Song, Formability of Al–Nb Bearing Ultra High-strength TRIP-aided Sheet Steels with Bainitic Ferrite and/or Martensite Matrix, ISIJ International, 50, No.1, 162-168, (2010).
 Dong-Woo Suh, Seong-Jun Park, Tae-Ho Lee, Chang-Seok Oh, Sung-Joon Kim, Influence of Al on the Microstructural Evolution and Mechanical Behavior of Low-Carbon, Manganese Transformation-Induced-Plasticity Steel, Metallurgical and Materials Transactions A, 41A, 397-408, (2010).
 Nobuhiro Tsuji , Susumu Okuno , Yuichiro Koizumi and Yoritoshi Minamino, Toughness of Ultrafine Grained Ferritic Steels Fabricated by ARB and Annealing Process, Materials Transactions, 45, No. 7, 2272-2281, (2004).
 Rika Yoda, Kosuke Shibata, Takatoshi Morimitsu, Daisuke Terada and Nobuhiro Tsuji, Formability of ultrafine-grained interstitial-free steel fabricated by accumulative roll-bonding and subsequent annealing, Scripta Materialia, 65, 175-178, (2011).  Book: Structural Nanocrystalline Materials Fundamentals and
Applications, Carl Koch, Ilya Ovid'ko, Sudipta Seal, Stan Veprek, Chapter 5 - Mechanical properties of structural nanocrystalline materials – theory and simulations, Cambridge Universtiy Press, Cambridge, 292, (2007).
 Jean-Pierre Birat, Steel’s Vision for the 2030s and Beyond: The Strategic Research Agenda of ESTEP, The European Steel Technology Platform, Seminars at MEFOS and Jernkontoret, Luleå & Stockholm, Sweden, 23-26, 1-18, (2013).
 Pekka Erkkilä, New solutions for automotive industry,
https://www.outokumpu.com/SiteCollectionDocuments/CMD-2015-Pekka-Erkkila.pdf, 1-16, (2015), [Accessed November 2016].  www.worldstainless.org, Railcars in Stainless Steel A Sustainable
Solution for Sustainable Public Transport, International Stainless Steel Forum, Brussels, Belgium, 1-9, (2010).
 Pierre-Jean Cunat, Stainless steel properties for structural automotive applications, Metal Bulletin International Automotive Materials Conference, Cologne, 1-10, (2000).
 Book: Mechanical Metallurgy, George E Dieter, Chapter 6 – Strengthening Mechanisms, McGraw Hill Book Company, SI Metric Edition, 184-240, (Second Edition, 1988).
 PhD Thesis: Dilip Chandrasekaran, Grain Size and Solid Solution Strengthening in Metals, Department of Materials Science and Engineering, Royal Institute of Technology, Sweden, 1-67, (2003).  L.P. Karjalainen, T. Taulavuori, M. Sellman, A. Kyröläinen, Some
Strengthening Methods for Austenitic Stainless Steels, Steel Research International, 79, No. 6, 404-412, (2008).
 Book: Fundamentals of Materials Science and Engineering, William D. Callister, Jr., Chapter 8 – Deformation and Strengthening Mechanisms, John Wiley & Sons, Inc., 197-219, Fifth Edition (2001).
 Book: Physical Metallurgy Principles, Robert E. Reed-Hill, Chapter 9- Precipitation Hardening, Litton Educational Publishing, Inc, 358-377, Second Edition (1973).
 Kaka Ma, Haiming Wen, Tao Hu, Troy D. Topping, Dieter Isheim, David N. Seidman, Enrique J. Lavernia, Julie M. Schoenung, Mechanical behavior and strengthening mechanisms in ultrafine grain precipitation-strengthened aluminum alloy, Acta Materialia, 62, 141-155, (2014).
 Book: Physical Foundations of Materials Science, G. Gottstein, Chapter 1- Recovery, Recrystallization, Grain Growth, Springer, 1-54, (2005).
 Book: Fundamentals of Materials Science, E.J. Mittemeijer, Chapter 10 - Recovery, Recrystallization and Grain Growth, Springer-Verlag Berlin Heidelberg, 463-496, (2010).
 I. Baker, Recovery, recrystallization and grain growth in ordered alloys, Intermetallics, 8, 1183-1196, (2000).
 Book: Automotive Plastics & Composites - Worldwide Markets & Trends to 2007, D. Mann, Chapter 5- Competitions between plastics and composites and other materials, Reinforced Plastic magazine, Elsevier Advanced Technology, 82, (2007).
 Atshushi Itami, Kohsaku Ushioda, Noritoshi Kimura, Hirohide Asano, Yoshitaka kimura, Kazuo Koyama, Development of new formable Cold rolled sheet steels For automobile body panels, Nippon Steel Technical Report No 64, 26, (1995).
 S. Hoile, Processing and properties of mild interstitial free steels- A Review, Materials science and technology, 16, 1079-1093, (2000).
 R. Rana, S.B. Singh, W. Bleck, and O.N. Mohanty, Effect of Temperature and Dynamic Loading on the Mechanical Properties of Copper-Alloyed High-Strength Interstitial-Free Steel, Metallurgical and Materials Transactions A, 40A, 856, (2009).  Takehide Senuma, Physical Metallurgy of Modern High Strength
Steel Sheets- A Review, ISIJ International, 41, No. 6, 520-532, (2001).
 R. Rana, W. Bleck, S.B. Singh, O.N. Mohanty, Development of high strength interstitial free steel by copper precipitation hardening, Materials Letters, 61, 2919-2922, (2007).
 Georgy J. Raab , Ruslan Z. Valiev , Terry C. Lowe , Yuntian T. Zhu , Continuous processing of ultrafine grained Al by ECAP– Conform, Materials Science and Engineering A, 382, 30-34, (2004).
 Kyung-Tae Park, Dong Hyuk Shin, Annealing behavior of submicrometer grained ferrite in a low carbon steel fabricated by severe plastic deformation, Materials Science and Engineering A, 334, 79-86, (2002).
 Nobuhiro Tsuji, Naoya Kamikawa, Rintaro Ueji, Naoki Takata, Hirofumi Koyama, Daisuke Terada, Managing Both Strength and Ductility in Ultrafine Grained Steels- A Review, ISIJ International, 48, No. 8, 1114-1121, (2008).
 Gencaga Purcek, Onur Saray, Ibrahim Karaman, and Hans J. Maier, High Strength and High Ductility of Ultrafine-Grained Interstitial-Free Steel Produced by ECAE and Annealing, Metallurgical and Materials Transactions A, 43A, 1884-1894, (2012).
 Onur Saray, Gencaga Purcek, Ibrahim Karaman, Hans J. Maier, Impact Toughness of Ultrafine-Grained Interstitial-Free Steel, Metallurgical and Materials Transactions A, 43A, 4320-4330, (2012).
 K. Dehghani and J.J. Jonas, Dynamic Bake Hardening of Interstitial-Free Steels, Metallurgical and Materials Transactions A, 31A, 1375-1384, (2000).
 M.M. Humane, R.K. Minj, D.R. Peshwe, and R.K. Paretkar, Texture and Formability of One-Step and Two-Step Cold-Rolled and Annealed Interstitial Free High-Strength Steel Sheets, Metallurgical and Materials Transactions A, 42A, 1692-1708, (2011).
 Woo Chang Jeong, Effect of Prestrain on Aging and Bake Hardening of Cold-Rolled, Continuously Annealed Steel Sheets, Metallurgical and Materials Transactions A, 29A, 463-467, (1998).  www.asminternational.org/Book: Alloying: Understanding the
Basics, Product Code: #06117G, Chapter: High Strength Low Alloy Steel, 193-202 [Accessed December 2016].
 M. Militzer, E.B. Hawbolt, T.R. Meadowcroft, Microstructural Model for Hot Strip Rolling of High-Strength Low-Alloy Steels, Metallurgical and Materials Transactions A, 31A, 1247-1259, (2000).
 E. V. Pereloma and J. D. Boyd, Effects of simulated on line accelerated cooling processing on transformation temperatures and microstructure in microalloyed steels Part 1 - Strip processing, Materials Science and Technology, 12, 808-817, (1996).
 M. Charleux, W.J. Poole, M. Militzer, A. Deschamps,
Precipitation Behavior and its effect on strengthening of an HSLA-Nb/Ti Steel, Metallurgical and Materials Transactions A, 32A, 1635-1647, (2001).
 Won-Beom Lee, Seung-Gab Hong, Chan-Gyung Park, Sung-Ho Park, Carbide Precipitation and High-Temperature Strength of Hot-rolled High-Strength, Low-Alloy Steels Containing Nb and Mo, Metallurgical and Materials Transactions A, 33A, 1689-1698, (2002).
 S. Shanmugam, R.D.K. Misra, T. Mannering, D. Panda , S.G. Jansto, Impact toughness and microstructure relationship in niobium- and vanadium-microalloyed steels processed with varied cooling rates to similar yield strength, Materials Science and Engineering A, 437, 436-445, (2006).
 S. Shanmugam, N.K. Ramisetti , R.D.K. Misra , T. Mannering , D. Panda , S. Jansto, Effect of cooling rate on the microstructure and mechanical properties of Nb-microalloyed steels, Materials Science and Engineering A, 460-461, 335-343, (2007).
 Davood Nakhaie, Pooya Hosseini Benhangi, Fateh Fazeli, Mohammad Mazinani, Ebrahim Zohour Vahid Karimi, Mahmoud Reza Ghandehari Ferdowsi, Controlled Forging of a Nb Containing Microalloyed Steel for Automotive Applications, Metallurgical and Materials Transactions A, 43A, p. 5209-5217, (2012).
 Hardy Mohrbacher, Niobium Microalloyed Automotive Sheet Steel – A Cost Effective Solution to the Challenges of Modern Body Engineering, International Symposium on Niobium Microalloyed Sheet Steel for Automotive Application, Edited by S. Hashimoto, S. Jansto, H. Mohrbacher, and F. Siciliano, TMS (The Minerals, Metals & Materials Society), 1-23, (2006).
Materials Science and Metallurgy Engineering 13
 Debanshu Bhattacharya, Microalloyed Steels for the Automotive Industry – A Review, Technological Metallurgical Materials Mineralogy, São Paulo, 11, No. 4, 371-383, (2014).
 S.K. Ghosh, P.S. Bandyopadhyay, S. Kundu, S. Chatterjee, Copper bearing microalloyed ultrahigh strength steel on a pilot scale: Microstructure and properties, Materials Science and Engineering A, 528, 7887-7894, (2011).
 Naoki Maruyama, Masaaki Sugiyama, Takuya Hara, Hiroshi Tamehiro, Precipitation and phase transformation of Cu particles in low alloy ferritic martensitic steels, Materials Transactions, JIM, 40, No. 4, 268-277, (1999).
 Stuart Keeler, Meenachem Kimchi, Advanced High strength Steels Application Guidelines Version 5.0, 1-276, Available at: http://www.autosteel.org, (2014), [Accessed December 2016].  Sota Goto , Chikara Kami , Shuji Kawamura, Effect of alloying
elements and hot-rolling conditions on microstructure of bainitic-ferrite/martensite dual phase steel with high toughness, Materials Science & Engineering A, 648, 436-442, (2015).
 Y. Mazaheri, A. Kermanpur, A. Najafizadeh, Microstructures, Mechanical Properties, and Strain Hardening Behavior of an Ultrahigh Strength Dual Phase Steel Developed by Intercritical Annealing of Cold-Rolled Ferrite/Martensite, Metallurgical and Materials Transactions A, 46A, 3052-3062, (2015).
 Gejza Rosenberg, Iveta Sinaiova, Pavol Hvizdos , L’ubosˇ Juhar, Development of Cold-Rolled Dual-Phase Steels with Tensile Strength Above 1000 MPa and Good Bendability, Metallurgical and Materials Transactions A, 46A, 4755-4771, (2015).
 M. Papa Rao, V. Subramanya Sarma, S. Sankaran, Processing of Bimodal Grain-Sized Ultrafine-Grained Dual Phase Microalloyed V-Nb Steel with 1370 MPa Strength and 16 pct Uniform Elongation Through Warm Rolling and Intercritical Annealing, Metallurgical and Materials Transactions A, 45A, 5313-5317, (2014).
 Yousef Mazaheri, Ahmad Kermanpur, Abbas Najafizadeh, Strengthening Mechanisms of Ultrafine Grained Dual Phase Steels Developed by New Thermomechanical Processing, ISIJ International, 55, No.1, 218-226, (2015).
 Lei Shi , Zesheng Yan , Yongchang Liu , Cheng Zhang , Zhixia Qiao , Baoqun Ning , Huijun Li, Improved toughness and ductility in ferrite/acicular ferrite dual-phase steel through intercritical heat treatment, Materials Science&Engineering A, 590, 7-15, (2014).  Mehdi Asadi, Georg Frommeyer, Ali Aghajani, Ilana Timokhina,
Heinz Palkowski, Local Laser Heat Treatment in Dual-Phase Steels, Metallurgical and Materials Transactions A, 43A, 1244-1258, (2012).
 Hamid Azizi-Alizamini, Matthias Militzer, Warren J. Poole, Formation of Ultrafine Grained Dual Phase Steels through Rapid Heating, ISIJ International, 51, No. 6, 958–964, (2011).
 Irina Pushkareva, Sébastien Allain, Colin Scott, Abdelkrim Redjaïmia, Antoine Moulin, Relationship between Microstructure, Mechanical Properties and Damage Mechanisms in High Martensite Fraction Dual Phase Steels, ISIJ International, 55, No.10, 2237-2246, (2015).
 Zhengzhi Zhao , Tingting Tong , Juhua Liang , Hongxiang Yin, Aimin Zhao , Di Tang, Microstructure, mechanical properties and fracture behavior of ultra-high strength dual-phase steel, Materials Science & Engineering A, 618, 182-188, (2014).
 Yousef Mazaheri , Ahmad Kermanpur,Abbas Najafizadeh, A novel route for development of ultrahigh strength dual phase steels, MaterialsScience & Engineering A, 619, 1-11, (2014).
 Yong-lin Kang , Qi-hang Han , Xian-meng Zhao , Ming-hui Cai, Influence of nanoparticle reinforcements on the strengthening mechanisms of an ultrafine-grained dual phase steel containing titanium, Materials and Design, 44, 331-339, (2013).
 Jun Hu, Lin-Xiu Du, Jian-Jun Wang, Cai-Ru Gao, Tong-Zi Yang, An-Yang Wang, R.D.K. Misra, Microstructures and Mechanical Properties of a New As-Hot-Rolled High-Strength DP Steel Subjected to Different Cooling Schedules, Metallurgical and Materials Transactions A, 44A, 4937-4946, (2013).
 M.D. Zhang, J.Hu, W.Q.Cao, H.Dong, Microstructure and mechanical properties of high strength and high toughness micro-laminated dual phase steels, Materials Science & Engineering A, 618, 168-175, (2014).
 Marion Calcagnotto, Dirk Ponge, Dierk Raabe, Effect of grain refinement to 1µm on strength and toughness of dual-phase steels, Materials Science and Engineering A, 527, 7832-7840, (2010).
 Hossein Hosseini-Toudeshky , Behnam Anbarlooie , Javad Kadkhodapour , Ghasem Shadalooyi, Microstructural deformation pattern and mechanical behavior analyses of DP600 dual phase steel, Materials Science & Engineering A, 600, 108-121, (2014).  Ilana Timokhina, Elena Pereloma, Peter Hodgson, The Formation
of Complex Microstructures After Different Deformation Modes in Advanced High-Strength Steels, Metallurgical and Materials Transactions A, 45A, 4247-4256, (2014).
 Product catalogue of Arcelormittal Automotive worldwide – European edition,
http://automotive.arcelormittal.com/saturnus/sheets/B_EN.pdf, 1-7, [Accessed December 2016].
 Y.F.Shen, Y.D.Liu, X.Sun, Y.D.Wang, L.Zuo, R.D.K.Misra, Improved ductility of a transformation-induced-plasticity steel by nanoscale austenite lamellae, Materials Science & Engineering A, 583, 1-10, (2013).
 Seyed Mohammad Kazem Hosseini , Abbass Zarei-Hanzaki , Steve Yue, Effects of ferrite phase characteristics on microstructure and mechanical properties of thermomechanically-processed low-silicon content TRIP-assisted steels, Materials Science & Engineering A, 626, 229-236, (2015).
 Bruno C. De Cooman, Paul Gibbs, Seawoong Lee, David K. Matlock, Transmission Electron Microscopy Analysis of Yielding in Ultrafine-Grained Medium Mn Transformation-Induced Plasticity Steel, Metallurgical and Materials Transactions A, 44A, 2563-2572, (2013).
 Koh-ichi Sugimoto, Muneo Murata, Sung-Moo Song, Formability of Al–Nb Bearing Ultra High-strength TRIP-aided Sheet Steels with Bainitic Ferrite and/or Martensite Matrix, ISIJ International, 50, No. 1, 162-168, (2010).
 Junya Kobayashi, Daiki Ina, Yuji Nakajima, Koh-Ichi Sugimoto, Effects of Microalloying on the Impact Toughness of Ultrahigh-Strength TRIP-Aided Martensitic Steels, Metallurgical and Materials Transactions A, 44A, 5006-5017, (2013).
 Qihang Han, Yulong Zhang, Li Wang, Effect of Annealing Time on Microstructural Evolution and Deformation Characteristics in 10Mn1.5Al TRIP Steel, Metallurgical and Materials Transactions A, 46A, 1917-1926, (2015).
 Haiwen Luo , Han Dong, New ultrahigh-strength Mn-alloyed TRIP steels with improved formability manufactured by intercritical annealing, Materials Science & Engineering A, 626, 207-212, (2015).
 Minghui Cai, Zhun Li, Qi Chao, Peter D. Hodgson, A Novel Mo and Nb Microalloyed Medium Mn TRIP Steel with Maximal Ultimate Strength and Moderate Ductility, Metallurgical and Materials Transactions A, 45A, 5624-5634, (2014).
 Chang Gil Lee, Sung-Joon Kim, Tae-Ho Lee, Chang-Seok Oh, Effects of Tramp Elements on Formability of Low-carbon TRIP aided Multiphase Cold-rolled Steel Sheets, ISIJ International, 44, No. 4, 737-743, (2004).
 Gianfranco Lovicu, Mauro Bottazzi, Fabio D’aiuto, Massimo De Sanctis, Antonella Dimatteo, Ciro Santus, Renzo Valentini, Hydrogen Embrittlement of Automotive Advanced High-Strength Steels, Metallurgical and Materials Transactions A, 43A, 4075-4087, (2012).
 Product catalogue of Arcelormittal Automotive worldwide – European edition,
http://automotive.arcelormittal.com/saturnus/sheets/C_EN.pdf, 1-9, [Accessed January 2017].
 Product catalogue of Arcelormittal Automotive worldwide – North American edition,
http://automotive.arcelormittal.com/repository2/AutomotivProduct %20offer/MartensiticSteels.pdf, 1-2, [Accessed January 2017].  George Kraus, Heat Treated Martensitic Steels: Microstructural
Systems for Advanced Manufacture, A Review, ISIJ International, 35, No. 4, 349-359, (1995).
 Hiroshi Matsuda, Reiko Mizuno, Yoshimasa Funakawa, Kazuhiro Seto, Saiji Matsuoka, Yasushi Tanaka, Effects of auto-tempering behaviour of martensite on mechanical properties of ultra high strength steel sheets, Journal of Alloys and Compounds, 577S, S661-S667, (2013).
 Product catalogue of Arcelormittal Automotive worldwide – European edition,
http://automotive.arcelormittal.com/saturnus/sheets/D_EN.pdf, 1-6, [Accessed January 2017].
 Haijiang Hu, Guang Xu, Li Wang, Zhengliang Xue, Yulong Zhang, Guanghui Liu, The effects of Nb and Mo addition on transformation and properties in low carbon bainitic steels, Materials and Design, 84, 95-99, (2015).
 Jun Hu , Lin-Xiu Du , Jian-Jun Wang, Effect of cooling procedure on microstructures and mechanical properties of hot rolled Nb–Ti bainitic high strength steel, Materials Science and Engineering A, 554, 79-85, (2012).
 F.G. Caballero, S. Allain, J. Cornide, J.D. Puerta Velásquez, C.Garcia-Mateo, M.K.Miller, Design of cold rolled and continuous annealed carbide-free bainitic steels for automotive application, Materials and Design, 49, 667-680, (2013).
 Francisca García Caballero, María Jesús Santofimia, Carlos Capdevila, Carlos García-Mateo, Carlos García De Andrés, Design of Advanced Bainitic Steels by Optimisation of TTT Diagrams and T0 Curves, ISIJ International, 46, No. 10, 1479-1488, (2006).
 Product catalogue of Arcelormittal Automotive worldwide – European edition,
http://automotive.arcelormittal.com/saturnus/sheets/E_EN.pdf, 1-9, [Accessed January 2017].
 W. J. Liu, An Introduction to Advanced Hot-Formed Steel for Automobile, Acta Metallurgica Sinicia (English Letter), 27, No. 3, 373-382, (2014).
 Hongsheng Liu, Wei Liu, Jun Bao, Zhongwen Xing, Baoyu Song, and Chengxi Lei, Numerical and Experimental Investigation into Hot Forming of Ultra High Strength Steel Sheet, Journal of Materials Engineering and Performance, 20, No.1, 1-10, (2011). R. George, A. Bardelcik, M.J. Worswick, Hot forming of boron
steels using heated and cooled tooling for tailored properties, Journal of Materials Processing Technology, 212, 2386-2399, (2012).
Book: New Trends and Developments in Automotive System Engineering, Edited by Marcello Chiaberge, Chapter 6 - High Mn TWIP Steels for Automotive Applications, B. C. De Cooman, Kwang-geun Chin and Jinkyung Kim, InTech Press, Cambridge, Shanghai , 101-128, (2011).
R. W. Neu, Performance and Characterization of TWIP Steels for Automotive Applications, Materials performance and characterization, 2, No.1, 244-284, (2013).
G.W. Yuan, M.X.Huang, Supper strong nanostructured TWIP steels for automotive applications, Progress in Natural Science: Materials International, 24, 50-55, (2014).
M. Daamen, O. Güvenç, M. Bambach, G. Hirt, Development of efficient production routes based on strip casting for advanced high strength steels for crash-relevant parts, CIRP Annals - Manufacturing Technology, 63, 265-268, (2014).
G. Dini, A. Najafizadeh, R. Ueji , S.M. Monir-Vaghefi, Improved tensile properties of partially recrystallized submicron grained TWIP steel, Materials Letters, 64, 15-18, (2010).
I.B. Timokhina, A.Medvedev, R.Lapovok, Severe plastic deformation of a TWIP steel, Materials Science & Engineering A, 593, 163-169, (2014).
Georg Frommeyer, Udo Brüx, Peter Neumann, Supra-Ductile and High-Strength Manganese-TRIP/TWIP Steels for High Energy Absorption Purposes, ISIJ International, 43, No. 3, 438-446, (2003).
Seok Su Sohn, Kayoung Choi, Jai-Hyun Kwak, Nack J. Kim, Sunghak Lee, Novel ferrite–austenite duplex lightweight steel with 77% ductility by transformation induced plasticity and twinning induced plasticity mechanisms, Acta Materialia, 78, 181-189, (2014).
John G. Speer, E. De Moor, K.O. Findley, D.K. Matlock, B.C. De Cooman, D.V. Edmonds, Analysis of Microstructure Evolution in Quenching and Partitioning Automotive Sheet Steel, Metallurgical and Materials Transactions A, 42A, 3591-3601, (2011).
A. Grajcar, R. Kuziak, W. Zalecki, Third generation of AHSS with increased fraction of retained austenite for the automotive industry, achieves of civil and mechanical engineering, 12, 334-341, (2012).
Hao Qu, Gary M. Michal, Arthur H. Heuer, Third Generation 0.3C-4.0Mn Advanced High Strength Steels Through a Dual Stabilization Heat Treatment: Austenite Stabilization Through
Paraequilibrium Carbon Partitioning, Metallurgical and Materials Transactions A, 45A, 2741-2749, (2014).
Eun Jung Seo, Lawrence Cho, Bruno Charles De Cooman, Application of Quenching and Partitioning (Q&P) Processing to Press Hardening Steel, Metallurgical and Materials Transactions A, 45A, 4022-4037, (2014).
M. Naderi, M. Abbasi, A. Saeed-Akbari, Enhanced Mechanical Properties of a Hot-Stamped Advanced High-Strength Steel via Tempering Treatment, Metallurgical and Materials Transactions A, 44A, 1852-1861, (2013).
Shengwei Qin, Yu Liu, Qingguo Hao, Ying Wang, Nailu Chen, Xunwei Zuo, Yonghua Rong, The Mechanism of High Ductility for Novel High-Carbon Quenching–Partitioning–Tempering Martensitic Steel, Metallurgical and Materials Transactions A, 46A, 4047-4055, (2015).
Santigopal Samanta, Sourav Das, Debalay Chakrabarti, Indradev Samajdar, Shiv Brat Singh, Arunansu Haldar, Development of Multiphase Microstructure with Bainite, Martensite, and Retained Austenite in a Co-Containing Steel Through Quenching and Partitioning (Q&P) Treatment, Metallurgical and Materials Transactions A, 44A, 5653-5664, (2013).
Tao Lin, Hong-Wu Song, Shi-Hong Zhang, Ming Cheng, Wei-Jie Liu, Yun Chen, Microstructure, Mechanical Properties, and Toughening Mechanisms of a New Hot Stamping-Bake Toughening Steel, Metallurgical and Materials Transactions A, 46A, 4038-4046, (2015).
Ken-ichi Ikeda, Nana Kwame Gyan Yamoah, William T. Reynolds Jr., Jun-Ichi Hamada, and Mitsuhiro Murayama, Effect of Laves Phase on High-Temperature Deformation and Microstructure Evolution in an 18Cr-2Mo-0.5Nb Ferritic Stainless Steel, Metallurgical and Materials Transactions A, 46A, 3460-3469, (2015).
W. Xu, P.E.J. Rivera-Diaz-del-Castillo, W. Yan, K. Yang, D. San Martin, L.A.I. Kestens, S. van der Zwaag, A new ultrahigh-strength stainless steel ultrahigh-strengthened by various coexisting nano precipitates, Acta Materialia, 58, 4067-4075, (2010).
Chang Ye, Abhishek Telang, Amrinder S. Gill, Sergey Suslov, Yaakov Idell, Kai Zweiacker, JörgM.K.Wiezorek, Zhong Zhou, Dong Qian, Seetha Ramaiah Mannava, Vijay K. Vasudevan, Gradient nanostructure and residual stresses induced by Ultrasonic Nano-crystal Surface Modification in 304 austenitic stainless steel for high strength and high ductility, Materials Science & Engineering A, 613, 274-288, (2014).
A. S. Hamada, A. P. Kisko, P. Sahu, L. P. Karjalainen, Enhancement of mechanical properties of a TRIP-aided austenitic stainless steel by controlled reversion annealing, Materials Science & Engineering A, 628, 154-159, (2015).
K. H. Lo, C. H. Shek,J. K. L. Lai, Recent developments in stainless steels, Materials Science and Engineering R, 65, 39-104, (2009).
S.V. Dobatkin, O. V. Rybalchenko, N. A. Enikeev, A. A. Tokar, M. M. Abramova, Formation of fully austenitic ultrafine-grained high strength state in metastable Cr–Ni–Ti stainless steel by severe plastic deformation, Materials Letters, 166, 276-279, (2016). Yi Xiong , Tiantian He , Junbei Wang , Yan Lu, Lufei Chen,
Fengzhang Ren, Yuliang Liu , Alex A. Volinsky, Cryorolling effect on microstructure and mechanical properties of Fe–25Cr– 20Ni austenitic stainless steel, Materials and Design, 88, 398-405, (2015).
A. Rezaee, A. Kermanpur, A. Najafizadeh, M. Moallemi, Production of nano/ultrafine grained AISI 201L stainless steel through advanced thermo-mechanical treatment, Materials Science and Engineering A, 528, 5025-5029, (2011).
R.D.K. Misra, X.L. Wan, V.S.A. Challa, M.C. Somani, L.E. Murr, Relationship of grain size and deformation mechanism to the fracture behavior in high strength–high ductility nano-structured austenitic stainless steel, MaterialsScience & Engineering A, 626, 41-50, (2015).
Guixun Sun, Yu Zhang, Shicheng Sun, Jiangjiang Hu, Zhonghao Jiang, Changtao Ji, Jianshe Lian, Plastic flow behavior and its relationship to tensile mechanical properties of high nitrogen nickel-free austenitic stainless steel, Materials Science & Engineering A, 662, 432-442, (2016).
Materials Science and Metallurgy Engineering 15
Seok Su Sohn, Hyejin Song, Byeong-Chan Suh, Jai-Hyun Kwak, Byeong-Joo Lee, Nack J. Kim, Sunghak Lee, Novel ultra-high-strength (ferrite + austenite) duplex lightweight steels achieved by fine dislocation substructures (Taylor lattices), grain refinement, and partial recrystallization, Acta Materialia, 96, 301-310, (2015). Fuqiang Yang, Renbo Song ⇑, Yaping Li, Ting Sun, Kaikun Wang,
Tensile deformation of low density duplex Fe–Mn–Al–C steel, Materials and Design, 76, 32-39, (2015).
P. Behjati, A. Kermanpur, A. Najafizadeh, H. Samaei Baghbadorani, J.-G. Jung, Y.-K.Lee, Influence of pre-cooling and deformation temperature on microstructure and mechanical properties in a high-manganese austenitic steel, Materials Science & Engineering A, 614, 232-237, (2014).
P. Behjati, A. Kermanpur, A. Najafizadeh, H. Samaei Baghbadorani, L.P. Karjalainen, J.-G. Jung,Y.-K. Lee, Design of a new Ni-free austenitic stainless steel with unique ultrahigh strength-high ductility synergy, Materials and Design, 63, 500-507, (2014).
S K Ghosh, P Mallick, P P Chattopadhyay, Effect of Cold Deformation on Phase Evolution and Mechanical Properties in an Austenitic Stainless Steel for Structural and Safety Applications, Journal of Iron and Steel Research, International, 19, No. 4, 63-68, (2012).
Iaroslava Shakhova, Andrey Belyakov, Zhanna Yanushkevich, Kaneaki Tsuzaki, Rustam Kaibyshev, On Strengthening of Austenitic Stainless Steel by Large Strain Cold Working, ISIJ International, 56, No. 7, 1289-1296, (2016).
Carola Celada Casero, David San Marti´n, Austenite Formation in a Cold-Rolled Semi-austenitic Stainless Steel, Metallurgical and Materials Transactions A, 45A, 1767-1777, (2014).
Hojjat Samaei Baghbadorani, Ahmad Kermanpur, Abbas Najafizadeh, Peiman Behjati, Mohammad Moallemi, Ahad Rezaee, Influence of Nb-Microalloying on the Formation of Nano/Ultrafine-Grained Microstructure and Mechanical Properties During Martensite Reversion Process in a 201-Type Austenitic Stainless Steel, Metallurgical and Materials Transactions A, 46A, 3406-3413, (2015).
Daniel M. Field, David C. Van Aken, Nanocrystalline Advanced High Strength Steel Produced by Cold Rolling and Annealing, Metallurgical and Materials Transactions A, 47A, 1912-1917, (2016).
Xiaodong Mao, Suk Hoon Kang, Tae Kyu Kim, Seul Cham Kim, Kyu Hwan Oh, Jinsung Jang, Microstructure and Mechanical Properties of Ultrafine-Grained Austenitic Oxide Dispersion Strengthened Steel, Metallurgical and Materials Transactions A, 47A, 5334-5343, (2016).
Qingxuan Ran, Wanjian Xu, Zhaoyu Wu, Jun Li, Yulai Xu, Xueshan Xiao, Jincheng Hu, Laizhu Jiang, Evolutions of Microstructure and Properties During Cold Rolling of 19Cr Duplex Stainless Steel, Metallurgical and Materials Transactions A, 47A, 5037-5048, (2016).
Yongcan Li, Wei Yan, James D. Cotton, Glamm J. Ryan, Yifu Shen, Wei Wang, Yiyin Shan, Ke Yang, A new 1.9 GPa maraging stainless steel strengthened by multiple precipitating species, Materials and Design, 82, 56-63, (2015).
M. Eskandari, A. Zarei-Hanzaki, M.A. Mohtadi-Bonab, Y.Onuki, R. Basu, A. Asghari, J.A. Szpunar, Grain-orientation-dependent of γ–€–α/ transformation and twinningin a super-high-strength,high
ductility austenitic Mn-steel, Materials Science & Engineering A, 674, 514-528, (2016).
Barna Roy, Rajesh Kumar , Jayanta Das, Effect of cryorolling on the microstructure and tensile properties of bulk nano-austenitic stainless steel, Materials Science & Engineering A, 631, 241-247, (2015).
M. Eskandari, A. Kermanpur, A. Najafizadeh, Formation of Nanocrystalline Structure in 301 Stainless Steel Produced by Martensite Treatment, Metallurgical and Materials Transactions A, 40A, 2241-2249, (2009).
Javad Mola, Bruno C. De Cooman, Quenching and Partitioning (Q&P) Processing of Martensitic Stainless Steels, Metallurgical and Materials Transactions A, 44A, 946-967, (2013).